- Nano Express
- Open Access
Temperature and Wavelength Dependence of Energy Transfer Process Between Quantized States and Surface States in CdSe Quantum Dots
Nanoscale Research Letters volume 12, Article number: 222 (2017)
Temperature and wavelength dependence of energy transfer (ET) process between quantized states and surface trap states of CdSe quantum dots was investigated, respectively. The experimental results demonstrate that the photoluminescence (PL) intensity of the quantized states decreases with respect to the trap state emission, especially at lower temperatures. The observed ET process between quantized states and trap states which is influenced by the thermal population behavior. At the same temperature, the silver films can greatly enhance the energy transfer (ET) rate from the quantized states to trap states due to surface plasmonic coupling effect.
Colloidal quantum dots (QDs) have displayed extensive applications for QD LEDs [1, 2], QD lasers [3–7], and QD solar cells [8–10]. For some applications, surface trap states of the QDs should be adequately suppressed to obtain high fluorescence efficiency of core quantized states. As a result, many researchers have employed various surface chemistry methods to eliminate surface emission . However, the surface state of QDs also plays an important role in photoluminescence (PL) quantum yield , photoluminescence (PL) lifetime , multi-exciton recombination [14–16], and optoelectronic processes [17–19]. Recently, some experimental results demonstrate that the emission of surface trap states with the wide visible light range can be applied to white LEDs [20–22]. Hu et al. have realized the fluorescent color tuning by post-synthesis thermal annealing method which enhances the PL intensity of surface trap states for CdSe QDs on polymethyl methacrylate (PMMA) silver films [23, 24].
However, the photoluminescence (PL) properties of surface states remain poorly understood with respect to our understanding of the quantized states. To elucidate the role of surface trap states, the surface state emission has been the focus of many investigations. Lifshitz et al. [25, 26] have confirmed the existence of recombination between shallow trapped electrons and deep trapped holes in the surface trap states of CdSe QDs by magnetic resonance. Wang et al. investigated the up-converted PL process of CdTe QDs at room temperature which confirms the existence of surface states . More importantly, Wang et al. further analyzed the photoluminescence (PL) dynamic process of surface states by time-resolved photoluminescence (PL) measurement at room temperature . We have reported that multi-excitons created in the quantized states can be effectively extracted to the acceptor trap states by utilizing an intrinsic energy transfer system in CdSe nanocrystals (NCs) . One can conclude that simple PL spectroscopy at room temperature does not reveal the nature of the surface states.
D. Kim et al. [30–33] have systematically reported the temperature effect on photoluminescence (PL) dynamics of the CdSe QDs, and the experimental result demonstrates that the bound-exciton state causes a significant impact on radiative decay lifetime. Temperature dependence of thermal population behavior is an important factor for the ET process from quantized states to surface states. However, researches paid little attention to the temperature-dependent dynamics of trap states and ET process between quantized states and trap states. The photoluminescence (PL) mechanism of trap states is being highly debated. Therefore, in order to better understand the photoluminescence (PL) origin of surface trap states in the CdSe QDs, it is important to explore temperature effect on photoluminescence (PL) decay and photoluminescence (PL) spectra of quantized states and surface trap states, respectively. Here, we investigate temperature and wavelength dependence of photoluminescence (PL) properties of surface states and ET process from low temperature to room temperature in this paper.
The CdSe quantum dots were diluted by toluene solution and the diluted CdSe quantum dot solution was added with PMMA powders on the scale of 30:1. In order to dissolve the PMMA powders, the mixed samples were placed in a dark room for several days. Then, the silicon wafer was deposited with 60-nm silver films by thermal evaporation method and the deposition film thickness was checked by the crystal thickness monitor. The PMMA–QD mixture was spin-coated on silicon wafer with 60-nm silver films at a speed of 3000 rpm. Consequently, the PMMA–QD silver film samples were prepared.
For PL spectral measurements, the 800-nm picosecond Ti: Sapphire laser with 76 MHz repetition rate was used to generate the 266-nm and 400-nm wavelength pulse laser based on second harmonic and third harmonic conversion technique, respectively. The 266-nm and 400-nm pulse lasers were focused onto the sample surface with a power density of ~100 W/cm2 at an incident angle of ~45°. The photoluminescence (PL) from samples was collected vertically by a 60× objective and sent to the spectrometer, and the emission photoluminescence (PL) spectra were recorded with a monochromator (Acton SP-2500i, 0.5 m, 150 lines mm−1 grating, blazed at 500 nm). For time-resolved PL decay measurements, the photoluminescence (PL) from the samples was collected by the same objective and then was detected by the single-photon counting system with the 250 ps time resolution. Temperature dependence of PL and lifetime measurements were performed in the liquid helium cryogenic system from low temperature to room temperature.
Results and Discussion
The PL spectra of quantized states and surface trap states for QDs on quartz coverslip at room temperature are shown in Fig. 1a, which consists of two peaks at 550 and 700 nm for the core quantized states and surface trap states, respectively. From the PL spectra, the PL intensity of quantized states is dominant and the PL intensity of trap states is weak. Figure 1b shows PL spectra of the quantized states and trap states for QDs on the silver films at room temperature which consists of two peaks at the wavelength 525 and 625 nm from the core quantized states and surface trap states, respectively. For QDs on the silver films, the QDs had been coated with PMMA films and then spin-coated on silicon wafer with 60-nm silver films, so that the PMMA films can prevent the energy transfer from quantum dots to silver films which causes the fluorescence quenching effect. As compared with the PL properties of the CdSe on quartz coverslip, the lower PL intensity of quantized states emission and the enhancement PL intensity of trap states emission for QDs on the silver films are observed, which can be attributed to the enhanced carrier recombination in trap states and the enhanced ET rate from the quantized states to the trap states due to plasmonic coupling effect on the corrugated silver films. From the absorption spectra, the PL intensity of trap states became obvious only when the excitation wavelength was tuned within the quantized absorption band and the small surface volume of trap states could prevent their efficient absorption transitions [34, 35]. Therefore, It can be concluded that the energy transfer process should be the origin of the activation energy.
To explicate the above steady-state PL measurements, the time-resolved PL measurements of quantized states and trap states were investigated, respectively. The PL decay curves of quantized states and trap states for CdSe QDs on the quartz coverslip and silver films are shown in Fig. 2. The lifetime decay curve of quantized state emission (green line) for CdSe QDs on the quartz coverslip is well fitted with double exponential functions which exhibit a fast component of 2.2 ns and a slow component of 21.1 ns. The fast component can be attributed to the intrinsic energy transfer process between quantized states and surface trap states. And the lifetime decay curve of trap states emission (black line) is fitted with single exponential function which only exhibits a slow component of 61.7 ns as shown in Fig. 2. However, the lifetime decay curve of quantized states emission (red curves) for CdSe on PMMA silver films with a slow component of 16.1 ns and a fast component of 1.6 ns and the lifetime decay curve of trap states emission (blue line) with 26.9 ns are shown in Fig. 2. By the above analysis, the relative faster component corresponds to ET lifetime between quantized states and trap states of semiconductor NCs, which strongly suggests that the surface states capture the excitons through the ET process , instead of direct carrier trapping or Auger-assisted carrier transfer through the multi-exciton ionization effect. According to above lifetime comparison, the PL lifetimes of quantized states and trap states on the PMMA silver films become shorter and the corresponding ET rate is greatly enhanced. The results demonstrate that the local surface plasmon from the QD/silver hybrid structures enhances trap state emission and accelerate ET process in QDs.
To further verify ET process from the quantized states to trap states inside QDs and eliminate ET process between QDs, we carried out time-resolved and spectrally resolved PL measurement within narrow spectral bands across the whole emission spectrum of quantized states for QDs in solution. The PL spectrum of CdSe QDs in solution is shown in Fig. 3a. However, the ET process between the QDs is absent in these diluted QD solutions due to the longer distance between the QDs. Figure 3b shows different wavelength PL decay curves of quantized states for CdSe QDs in solution. The PL decay curves were measured at the several emission peaks with 10 nm spectral width for CdSe QDs in solution. The lifetime decay curves are well fitted with double exponential functions which exhibit the fast component of 2.11, 2.25, 2.33, 2.37, and 2.41 ns at the peak value of wavelength 530, 540, 550, 560, and 570 nm, respectively. The results clearly demonstrate that the ET dynamic process is not homogeneous between quantized states and surface trap states, and the exciton decay lifetimes of quantized states become slower from the shorter wavelength to the longer wavelength. It is consistent with the nature of the spectral overlap between the different QDs : for this ET process, the shorter wavelength has a better spectral overlap than the longer wavelength and thus exhibits faster energy transfer process. The spectral dependence of the ET rate is in reasonably good agreement with the steady-state PL measurements. The wavelength-dependent PL decay curves provide clear evidence that the efficient ET process occurs inside the CdSe QDs.
Temperature dependence of thermal population behavior is an important factor for the ET process from quantized states to surface states. In order to understand the PL mechanism of surface trap states, it is necessary to systematically investigate temperature effect on PL spectra and PL decay of quantized states and surface trap states, respectively. Figure 4a shows the PL spectra of quantized states and surface trap states for CdSe QDs on quartz coverslip with different temperatures (4, 100, and 200 K), respectively. From these results, the PL intensity of quantized states decreases and the blue shift is observed at low temperature (4 K), which can be explained by the temperature dependence of band gap. However, the PL intensity of trap states increases by decreasing the temperature from 200 to 4 K for CdSe QDs on quartz coverslip. Figure 4b shows the PL spectra of CdSe QDs on PMMA silver films at different temperatures (4, 100, and 200 K), respectively. Therefore, the PL measurement typically reveals that the PL intensity of surface states increases at low temperature with respect to the PL intensity of quantized states. This observation suggests that thermal population behavior causes an important impact on the fluorescence emission of surface trap states and quantized states. The red-shift indicates an evidence for the occurrence of ET process between quantized states and trap states. Moreover, ET rate is not only influenced by the dipole strengths but also influenced by wave function overlaps between the donors and acceptors. However, the two influence factors are temperature dependence. At lower temperatures, the radiative recombination rates and nonradiative recombination rates in quantized states and trap states are remarkably suppressed. Therefore, the decreased ET rate at the lower temperature qualitatively explains the decreased spectral overlap and dipole strength of the excitonic emission of QDs.
To elaborate temperature effect on PL intensity of quantized states and trap states, we compare PL intensity of quantized states with that of trap states for CdSe on the quartz coverslip and silver films, respectively. The integrated PL intensity ratio of quantized states and trap states run up to 7.1 and 23 for CdSe QDs on the quartz coverslip surface and silver films at lower temperature (4 K) as shown in Fig. 4c, respectively. From the ratio of PL intensities of quantized states and trap states, it can be concluded that the silver films further enhance the energy transfer (ET) process from the quantized states to trap states due to the surface plasmonic coupling effect. To elucidate the temperature effect on energy transfer process from quantized states to surface states, the energy transfer model consisting of core quantized state, surface state, and ground state was established .
In Fig. 4d, we also plot integrated PL intensities of quantized state emission for CdSe on the quartz coverslip with different excitation power. Under high-power excitation, the quantized states can absorb multiple photons and generate multiple excitons per quantized state. More importantly, the saturation power for the quantized state emission decreases with lowering the temperature to 100 K. Therefore, more excitons generated with high excitation power in quantized states easily move to surface trap states by ET process at lower temperature. Compared the PL spectra of CdSe QDs on quartz coverslip with that of CdSe QDs on the silver films, these results obviously indicate the occurrence of the ET process from the quantized states to surface trap states as a function of temperature and ET rate is obviously enhanced due to the surface plasmonic coupling effect as shown in Fig. 4b.
In order to investigate the temperature effect on surface states, the observed temperature-dependent PL lifetimes were monitored by the time-resolved PL measurements. Figure 5a, b shows the temperature-dependent PL decay curves of quantized states and trap states on the quartz coverslip at 4, 100, and 200 K, respectively. The PL decay curves with biexponential components consisting of radiative decay and nonradiative decay were observed. The PL lifetimes of quantized states emission can be obtained by fitting τ 1 and τ 2 that correspond to the slow and fast component as shown in Fig. 5a. The difference between these components is obvious at 200 K with τ 1 = 22.1 ns and τ 2 = 0.34 ns. As the temperature is lowered to 100 K, there is a slight change in the fast component (~0.46 ns). And the slow component with a lifetime of τ 1 = 25.1 ns and the fast component with a lifetime of τ 2 = 0.51 ns are observed by further cooling to 4 K. By comparing with PL lifetime of quantized states emission, the PL lifetime (~65.1 ns) of trap states can be mainly regarded as radiative decay rate due to the negligence of thermal quenching effect.
The different PL decay curves of the quantized states emission and trap states emission can be fitted as shown in Fig. 5c, d. As can be seen from the two figures, the nonradiative decay rate becomes larger at 200 K and thus, the PL decay of quantized states is faster. However, the corresponding PL decay of trap states becomes slower at lower temperature. As mentioned above, the conventional three-state model can perfectly explain the temperature effect on PL dynamic process between quantized states and surface trap states [38, 39]. Therefore, the temperature-dependent PL intensity of quantized states and surface trap states as shown in Fig. 4a, b suggests the energy transfer that occurs through thermally activated process.
The temperature and wavelength dependence of energy transfer process between quantized states and trap states of CdSe QDs has been investigated by measuring PL spectra and PL decay on the quartz coverslip surface and silver films, respectively. The normalized PL intensity of the quantized states decreases at the lower temperature with respect to the trap state emission. And the enhanced ET process occurs from the quantized states to the surface trap states within the CdSe QDs, especially for CdSe QDs on the silver films at lower temperature. It can be concluded that the enhanced ET process attributes to plasmonic coupling effect at the lower temperature region and temperature dependence of thermal population behavior also plays an important role in the ET rate, especially for lower temperature.
Coe S, Woo WK, Bawendi MG, Bulovic V (2002) Electroluminescence from single monolayers of nanocrystals in molecular organic devices. Nature 420:800–803
Tessler N, Medvedev V, Kazes M, Kan SH, Banin U (2002) Efficient near-infrared polymer nanocrystal light-emitting diodes. Science 295:1506
Thompson BJ, Klimov VI (2003) Semiconductor and metal nanocrystals[M]
Klimov VI, Mikhailovsky AA, Xu S, Malko A, Hollingsworth JA, Leatherdale CA, Eisler HJ, Bawendi MG (2000) Optical gain and stimulated emission in nanocrystal quantum dots. Science 290:314
Kambhampati P (2011) Unraveling the structure and dynamics of excitons in semiconductor quantum dots. Acc Chem Res 44:1
Cooney RR, Sewall SL, Sagar DM, Kambhampati P (2009) State-resolved manipulations of optical gain in semiconductor quantum dots: size universality, gain tailoring, and surface effects. J Chem Phys 131:164706
Cooney RR, Sewall SL, Sagar DM, Kambhampati P (2009) Gain control in semiconductor quantum dots via state-resolved optical pumping. Phys Rev Lett 102:127404
Nozik AJ (2002) Quantum dot solar cells. Phys E 14:115
Gur I, Fromer NA, Geier ML, Alivisatos AP (2005) Air-stable all-inorganic nanocrystal solar cells processed from solution. Science 310:462
Greenham NC, Peng X, Alivisatos AP (1996) Charge separation and transport in conjugated-polymer/semiconductor-nanocrystal composites studied by photoluminescence quenching and photoconductivity. Phys Rev B 54:17628
Kortan AR, Hull R, Opila RL, Bawendi MG, Steigerwald ML, Carroll PJ, Brus LE (1990) Nucleation and growth of cadmium selendie on zinc sulfide quantum crystallite seeds, and vice versa, in inverse micelle media. J Am Chem Soc 112:1327
Kuno M, Lee JK, Dabbousi BO, Mikulec FV, Bawendi MG (1997) The band edge luminescence of surface modified CdSe nanocrystallites: Probing the luminescing state. J Chem Phys 106:9869
Garrett MD, Bowers MJ, McBride JR, Orndorff RL, Pennycook SJ, Rosenthal SJ (2008) Band edge dynamics in CdSe nanocrystals observed by ultrafast fluorescence upconversion. J Phys Chem C 112:436
Kambhampati P (2011) Hot exciton relaxation dynamics in semiconductor quantum dots: radiationless transitions on the nanoscale. J Phys Chem C 115:22089
Tyagi P, Kambhampati P (2011) False multiple exciton recombination and multiple exciton generation signals in semiconductor quantum dots arise from surface charge trapping. J Chem Phys 134:094706
McGuire JA, Sykora M, Joo J, Pietryga JM, Klimov VI (2010) Apparent versus true carrier multiplication yields in semiconductor nanocrystals. Nano Lett 10:2049
Galland C, Ghosh Y, Steinbruck A, Sykora M, Hollingsworth JA, Klimov VI, Htoon H (2011) Two types of luminescence blinking revealed by spectroelectrochemistry of single quantum dots. Nature 479:203
Rosen S, Schwartz O, Oron D (2010) Transient fluorescence of the off state in blinking CdSe/CdS/ZnS semiconductor nanocrystals is not governed by Auger recombination. Phys Rev Lett 104:157404
Bowers MJI, McBride JR, Garrett MD, Sammons JA, Dukes ADI, Schreuder MA, Watt TL, Lupini AR, Pennycook SJ, Rosenthal SJ (2009) Structure and ultrafast dynamics of white-light-emitting CdSe nanocrystals. J Am Chem Soc 131:5730
Schreuder MA, Xiao K, Ivanov IN, Weiss SM, Rosenthal SJ (2010) White light-emitting diodes based on ultrasmall CdSe nanocrystal electroluminescence. Nano Lett 10:573–576
Baker DR, Kamat PV (2010) Tuning the emission of CdSe quantum dots by controlled trap enhancement. Langmuir 26:11272
Bowers MJ, McBride JR, Rosenthal SJ (2005) White-light emission from magic-sized cadmium selenide nanocrystals. J Am Chem Soc 127:15378
Hu L, Wu HZ, Wan ZF, Cai CF, Xu TN, Lou TG et al (2012) Physical approaches to tuning the luminescence color patterns of colloidal quantum dots. New J Phys 14:013059
Hu L, Wu HZ, Du LX, Ge HY, Chen X, Dai N (2011) The effect of annealing and photoactivation on the optical transitions of band-band and surface trap states of colloidal quantum dots in PMMA. Nanotech 22:125202
Lifshitz E, Dag I, Litvin ID, Hodes G, Gorer S, Reisfeld R et al (1998) Optical properties of CdSe nanoparticle films prepared by chemical deposition and sol-gel methods. Chem Phys Lett 288:188–196
Lifshitz E, Dag I, Litvitn ID, Hodes G (1998) Optically detected magnetic resonance study of electron/hole traps on CdSe quantum dot surfaces. J Phys Chem B 102:9245–9250
Wang X, Yu WW, Zhang J, Aldana J, Peng X, Xiao M (2003) Photoluminescence upconversion in colloidal CdTe quantum dots. Phys Rev B 68:125318
Wang X, Qu L, Zhang J, Peng X, Xiao M (2003) Surface-related emission in highly luminescent CdSe quantum dots. Nano Lett 3:1103
Xu QF, Huang XN, Hua Z, Hu L, Du LX, Wu HZ et al (2016) Extended storage of multiple excitons in trap states of semiconductor nanocrystals. Appl Phys Lett 108:093110
Valerini D, Cretí A, Lomascolo M (2005) Temperature dependence of the photoluminescence properties of colloidal CdSe/ZnS core/shell quantum dots embedded in a polystyrene matrix. Phys Rev B 71:235409
Kim D, Yokota H, Shimura K, Nakayama M (2013) Temperature dependence of photoluminescence dynamics of self-assembled monolayers of CdSe quantum dots: the influence of the bound-exciton state. Phys Chem Chem Phys 15:21051
Yokota H, Okazaki K, Shimura K, Nakayama M, Kim D (2012) Photoluminescence properties of self-assembled monolayers of CdSe and CdSe/ZnS quantum dots. J Phys Chem C 116:5456–5459
Yokota H, Shimura K, Nakayama M, Kim D (2012) Optical properties of self-assembled monolayer of CdSe quantum dots. Phys Status Solidi C 9:2465–2468
Mooney J, Krause MM, Saari JI, Kambhampati P (2013) Challenge to the deep-trap model of the surface in semiconductor nanocrystals. Phys Rev B 87:081201
Chuang CH, Doane TL, Lo SS, Scholes GD, Burda C (2011) Measuring electron and hole transfer in core/shell nanoheterostructures. ACS Nano 5:6016
Kagan CR, Murray CB, Nirmal M, Bawendi MG (1996) Electronic energy transfer in CdSe quantum dot solids. Phys Rev Lett 76:1517
Crooker SA, Hollingsworth JA, Tretiak S, Klimov VI (2002) Spectrally resolved dynamics of energy transfer in quantum-dot assemblies: towards engineered energy flows in artificial materials. Phys Rev Lett 89:186802
Kim D, Okazaki K, Nakayama M (2009) Temperature dependence of the energy transfer of exciton states in bilayer structures of CdSe/ZnS quantum dots. Phys Rev B 80:045322
Labeau O, Tamarat P, Lounis B (2003) Temperature dependence of the luminescence lifetime of single CdSe/ZnS quantum dots. Phys Rev Lett 90:257404
This work was supported by the National Science Foundation of China under Grant No. 61307067 and No.11574125, the Science Foundation of Shandong Province under Grant No. ZR2015JL024, the Taishan Scholar Project of Shandong Province under Grant No. ts201511055, and the Fundamental Research Funds for the Central Universities under Grant No. 30920130129625.
QFX and CLY conceived and designed the experiments. LZ, LBK, and MLL prepared the samples. MMJ, HFM, DHW, and JNC performed the optical experiments. QFX and CLY co-wrote the manuscript. All authors read and approved the final manuscript.
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Zhang, L., Xu, Q., Liu, M. et al. Temperature and Wavelength Dependence of Energy Transfer Process Between Quantized States and Surface States in CdSe Quantum Dots. Nanoscale Res Lett 12, 222 (2017). https://doi.org/10.1186/s11671-017-1971-6
- Quantum dots
- Quantized states
- Surface trap states
- Energy transfer (ET)